Functionality in Electrospun Nanofibrous Membranes Based ... ... network assemblies (nanofibrous...
Embed Size (px)
Transcript of Functionality in Electrospun Nanofibrous Membranes Based ... ... network assemblies (nanofibrous...
Membranes 2011, 1, 249-264; doi:10.3390/membranes1030249
membranes ISSN 2077-0375
Functionality in Electrospun Nanofibrous Membranes Based on Fiber’s Size, Surface Area, and Molecular Orientation
Hidetoshi Matsumoto * and Akihiko Tanioka *
Department of Organic and Polymeric Materials, Tokyo Institute of Technology, 2-12-1 Ookayama, Meguro-ku, Tokyo 152-8552, Japan
* Authors to whom correspondence should be addressed; E-Mails: firstname.lastname@example.org (H.M.); email@example.com (A.T.); Tel.: +81-3-5734-2426; Fax: +81-3-5734-2876.
Received: 21 June 2011; in revised form: 15 August 2011 / Accepted: 16 August 2011 / Published: 26 August 2011
Abstract: Electrospinning is a versatile method for forming continuous thin fibers based on an electrohydrodynamic process. This method has the following advantages: (i) the ability to produce thin fibers with diameters in the micrometer and nanometer ranges; (ii) one-step forming of the two- or three-dimensional nanofiber network assemblies (nanofibrous membranes); and (iii) applicability for a broad spectrum of molecules, such as synthetic and biological polymers and polymerless sol-gel systems. Electrospun nanofibrous membranes have received significant attention in terms of their practical applications. The major advantages of nanofibers or nanofibrous membranes are the functionalities based on their nanoscaled-size, highly specific surface area, and highly molecular orientation. These functionalities of the nanofibrous membranes can be controlled by their fiber diameter, surface chemistry and topology, and internal structure of the nanofibers. This report focuses on our studies and describes fundamental aspects and applications of electrospun nanofibrous membranes.
Keywords: nanofiber; membrane; electrospinning; nanosize effect; high surface area; molecular orientation
Membranes 2011, 1
Ultrafine fibers, called “nanofibers” are a unique nanomaterial because of the nanoscaled dimensions in the cross-sectional direction and the macroscopic length of the fiber axis (see Figure 1). Therefore, nanofibers have both the advantages of functionality due to their nanoscaled structure and the ease of manipulation due to their macroscopic length. In addition, three-dimensional nanofiber network assemblies (nanofibrous membranes or fabrics) provide good mechanical properties and good handling characteristics.
Electrospinning is a versatile method based on an electrohydrodynamic process for forming continuous thin fibers ranging from several nanometers to tens of micrometers and can be used for the one-step forming of thin fibrous membranes [1–5]. The variety of materials, such as the polymer-solvent systems and polymerless sol-gel systems can be electrospun . Electrospun nanofibrous membranes with high surface areas have drawn significant attention for their practical applications, such as high-performance filter media, protective clothes, composites, drug delivery systems, scaffolds for tissue engineering, sensors, and electronic devices [2–5]. The functionalities of the nanofibers or nanofibrous membranes are based on their nanoscaled-size, high specific surface area, and high molecular orientation, and they can be controlled by their fiber diameter, surface chemistry and topology, and internal structure of the nanofibers. In addition, processing innovations to improve not only the controlling of morphologies but also the production capacity of electrospun nanofibers and nanofibrous membranes are in progress. In particular, the high-throughput electrospinning systems are an ongoing development (e.g., multi-needle and needleless processes) .
This review describes our fundamental studies on controlling of fiber diameter, surface chemistry and topology, and internal structure of the nanofibers by electrospinning and highlights our efforts toward the applications of nanofibrous membranes such as ion-exchangers, air filters, and antimicrobial materials.
Figure 1. Characteristics of nanofiber and nanofibrous membrane.
cross-sectional direction nanoscale (~nm)
fiber-axis direction macroscale (>cm)
- nanosize effect - superhigh surface area effect - molecular orientation effect
ease of handling D
D < 100 nm (practically 1μm) and
L/D > 100
Definition of Nanofiber Nanofibrous membrane
highly porous 3D-network structure
Membranes 2011, 1
2. Control of Structure of Nanofibers and Nanofibrous Membranes
2.1. Control of Size, Internal Structure, and Surface of Nanofiber
Many material parameters and process parameters have important effects on both the electrospinning process and the resulting fiber morphology . The fiber diameter depends on the solution properties (e.g., viscosity, conductivity, surface tension, permittivity, and boiling point) and/or operating conditions (e.g., applied voltage, spinneret-to-collector distance, and flow rate) summarized in Table 1.
Table 1. Control parameters for morphology and diameter of electrospun fibers (Adapted from ).
Solution properties Viscosity (molecular weight of polymer and concentration) Electric conductivity Solvent properties (surface tension, boiling point, polarity, and permittivity)
Operating conditions Applied voltage (typically from several kV to several 10 kV) Distance between spinneret and collector (typically from several cm to 50 cm) Feeding rate of polymer solution Spinneret (inner diameter, shape, and material)
Surrounding conditions Temperature Humidity
Practically, the viscosity and electric conductivity of the spinning solutions are crucial factors for controlling the fiber diameter. Figure 2 shows the typical effects of the solution viscosity and conductivity on the diameter of the electrospun fibers . In Figure 2a, the solution viscosity was changed by polymer concentration and the more viscous solution tends to form a thicker fiber. The increase in the entanglement of polymer chains caused by increasing the polymer concentration and/or molecular-weight of the polymer contributes to the formation of the fibrous structure. In addition, higher-molecular-weight polymers improve the electrospinnability from the lower viscosity solution and are effectively fabricated into thinner and homogenous fibers by electrospinning . The fiber diameter also decreases with an increase in the solution conductivity due to the addition of a small number of electrolytes (Figure 2b, pyridine and sodium carbonate were used as the organic and inorganic electrolytes, respectively). The adequate conductivity solution enhances electrostatic repulsion force on the surface of the jet during electrospinning, and consequently, the fiber diameter decreases . However, the high-conductivity solution prevents electric-field induced charging of the solution, and consequently show a low electrospinnability.
Membranes 2011, 1
Figure 2. (a) Effect of solution viscosity on the diameters of the electrospun phenolic-resin fibers. Solution viscosity was changed by polymer concentration. (b) Effect of solution conductivity on diameters of the electrospun phenolic-resin fibers. Additives to the spinning solution are pyridine and sodium carbonate (Adapted from ).
0 20 40 60 80 100 120
Viscosity / mPa sec
er / μ
0 5 10 15 20
er / μ
Conductivity / mS m-1
Many properties of the nanofibers, such as the mechanical, electrical, and optical properties depend not only on the intrinsic properties of a polymer, but also on the internal structure of the fibers. Therefore, control of the internal structure and molecular orientation of the nanofibers has been required for improvement of their properties. Recently, some researchers reported that electrospinning is a useful process for controlling the crystal morphology and molecular orientation of poly(ethylene oxide) (PEO) and polyoxymethylene (POM) nanofibers [11,12]. Our previous study also showed that the electrospun poly(vinylidene fluoride) (PVDF) nanofiber has an oriented crystalline region (the polar β-phase crystal is dominant) along the fiber axis . In addition, we reported that the formation and orientation of the ordered structure in the electrospun liquid crystalline polymer (LCP) fibers could be controlled by the fiber diameter during electrospinning . Figure 3 shows the wide-angle X-ray diffraction (WAXD) patterns of the uniaxially aligned electrospun LCP (main-chain LC polyester, BB-5(3-Me)) fibers with various diameters. The patterns include two sharp reflections with smectic layer spacings of 24.0 and 17.0 Å. The reflection patterns are ring-shaped for the thickest fiber with the diameter (D) = 4.71 µm (Figure 3a), and the sharp reflections are concentrated on the meridian for the thinner fibers (Figures 3b–d). The concentrated reflections indicate that the layer normal of the smectic layer is arranged parallel to the fiber axis in the electrospun LCP fibers. The clearest reflections were found for the fiber with D = 0.69 µm (Figure 3c). On the other hand, such clear reflections have not been obser